N A N O E X P R E S S
Electrodeposition of platinum and silver into
chemically modified microporous silicon
Ryo Koda, Kazuhiro Fukami*
, Tetsuo Sakka and Yukio H Ogata
Electrodeposition of platinum and silver into hydrophobic and hydrophilic microporous silicon layers was
investigated using chemically modified microporous silicon electrodes. Hydrophobic microporous silicon enhanced the electrodeposition of platinum in the porous layer. Meanwhile, hydrophilic one showed that platinum was hardly deposited within the porous layer, and a film of platinum on the top of the porous layer was observed. On the other hand, the electrodeposition of silver showed similar deposition behavior between these two chemically modified electrodes. It was also found that the electrodeposition of silver started at the pore opening and grew toward the pore bottom, while a uniform deposition from the pore bottom was observed in platinum electrodeposition. These electrodeposition behaviors are explained on the basis of the both effects, the difference in overpotential for metal deposition on silicon and on the deposited metal, and displacement deposition rate of metal.
Keywords:microporous silicon, noble metal, electrodeposition, hydration property
Porous silicon has some properties such as high specific surface area and semiconductivity which allow metal elec-trodeposition within the porous layer without special treatment. Such properties are advantageous to the prep-aration of metal/semiconductor hybrid materials and catalyst-dispersed porous structures. However, there is a difficulty in metal electrodeposition within porous silicon that plugging often occurs before it is fully and/or homo-geneously filled with metal [1-4]. Inhibition of plugging during metal deposition is indispensable for controlling the filling of metal by electrodeposition. For macroporous silicon, it was reported that the plugging often occurred in some metal deposition systems due to a high rate of dis-placement deposition which preferentially occurred at the pore opening and electrodeposition preferentially pro-ceeded on the deposits . Such an effect is not observed in the case of microporous silicon having hydrophobic pore wall, although the diameter of microporous silicon is much smaller than that of macroporous silicon. Another mechanism, which is different from the case of macropor-ous silicon, seems to control the deposition behavior in
microporous silicon. Recently, we have found that the hydrophobic and hydrophilic properties of microporous silicon have strong effects on the platinum electrodeposi-tion . Only the hydrophobic microporous silicon accel-erates the platinum deposition in the porous layer. Considering the surface hydration effect of platinum com-plex ions in the porous layer could explain this behavior.
In this study, electrodeposition behaviors of platinum and silver in chemically modified hydrophobic and hydro-philic microporous silicon are compared. The hydropho-bic property of microporous silicon has a strong effect on platinum electrodeposition, while the silver electrodeposi-tion is not affected by the hydrophobic and hydrophilic properties. The growth modes of the deposits show a clear difference between platinum and silver. These behaviors are explained on the basis of the both effects, the differ-ence in overpotential for platinum and silver electrodepo-sition on silicon, and the difference in displacement deposition rate between platinum and silver.
Two types of microporous silicon having various pore depths were prepared by anodization.p-type silicon (100)
Institute of Advanced Energy, Kyoto University, Uji, Kyoto 611-0011, Japan
with a resistivity of 10 to 20Ωcm was used. A mixture of 22 wt.% hydrogen fluoride/ethanol solution (47 wt.% hydrogen fluoride aqueous solution:ethanol = 1:1.7 in vol-ume) was used for the electrolyte. Anodization was carried out for 20 and 60 min at 2 mA cm−2. The depth of micro-porous structure was ca. 2 and 7μm, which was controlled by the duration of anodization. When the sample was ano-dized for 60 min under this condition, the microporous structure showed a macropore-like structure filled with microporous silicon . We call this structure ‘skeleton structure.’ After anodization, microporous silicon sub-strates were immersed for 15 h in n-hexane containing 0.2 M methyl propiolate and 0.2 M propiolic acid to make the pore wall hydrophobic and hydrophilic by hydrosilyla-tion reachydrosilyla-tion, respectively .
Platinum and silver were electrodeposited on the chemically modified microporous silicon electrodes. A platinum rod was used as the counter electrode. Plat-inum electrodeposition was carried out using 0.1 M K2PtCl4+ 0.5 M NaCl solution, and silver electrodeposi-tion was carried out using 0.1 M AgNO3+ 0.5 M KNO3 solution. Current density for the electrodeposition was set at a constant value of−6.4μA cm−2in all the cases.
Current density-potential (i-E) curves were measured. A platinum plate, barep-type silicon, and chemically modi-fied p-type silicon were used as the working electrodes, where plain silicon was employed without porosification. The counter electrode was a platinum rod, and the refer-ence electrode was an Ag/AgCl saturated KCl electrode. Scan rate of potential was set at 10 mV s−1.
A scanning electron microscope (JSM-6500 F, JEOL Ltd., Tokyo, Japan) was employed to obtain secondary electron images (SEI) and back scattered electron images (BEI) of the cross-sectional microporous silicon after metal electrodeposition. SEI illustrates the morphology. On the other hand, BEI provides atomic number con-trast: platinum and silver deposits appear brighter than silicon in the images.
Characterization of platinum and silver bath
i-E curves were measured to understand the electrode-position behavior of the platinum and silver baths on various electrodes. Figure 1 indicates that the i-Ecurves measured with flat silicon modified by the propiolic acid and methyl propiolate in both solutions are similar in shape. These results show that the difference in over-potential between the chemically modified silicon elec-trodes is not large for platinum electrodeposition. Compared to the platinum plate, the i-E curves of the chemically modified flat silicon shift to negative potential in the platinum bath (Figure 1a). As a result, higher
overpotential is necessary at the chemically modified sili-con compared with the platinum plate.
The i-E curves measured in silver bath behave at two differently modified silicon electrodes like the platinum case (Figure 1b). However, unlike the platinum case, a shift to negative potential is very small at the silicon electrodes. The result suggests that, in case of silver, the silicon elec-trodes do not require a higher overpotential than in the case of platinum.
Metal electrodeposition in chemically modified microporous silicon[image:2.595.307.539.90.479.2]
Platinum and silver electrodeposition was carried out for chemically modified microporous silicon with the depth
of 2μm. The cross-sectional images of microporous sili-con after electrodeposition of platinum are shown in Figure 2a,b. When the pore wall is hydrophilic, platinum is deposited only on the top of microporous silicon. On the other hand, when the pore wall is hydrophobic, plat-inum is deposited inside microporous silicon as reported elsewhere .
However, when silver electrodeposition was carried out, deposition proceeds uniformly both in the chem-ically modified hydrophobic and hydrophilic micropor-ous silicon (Figure 2c,d). Electrodeposition of silver is hard to be affected by the hydration properties of pore wall, such as hydrophobic or hydrophilic.
Time development of silver electrodeposition
To investigate the reason why the hydrophobic and hydrophilic properties of microporous silicon do not affect the electrodeposition behavior of silver, time de-velopment of silver electrodeposition in a chemically modified hydrophobic microporous silicon with the pore depth of ca. 7 μm was studied. Figures 3 and 4 show cross-sectional views of the samples after tion for 1 and 2 min, respectively. After electrodeposi-tion for 1 min, silver is deposited from the pore opening to the middle depth of the pore, which is independent of hydrophobic and hydrophilic properties. After 2-min electrodeposition, silver is uniformly deposited in both microporous silicon. The uniform deposition is also in-dependent of hydrophobic and hydrophilic properties. These results show that silver deposition proceeds from
the pore opening to the pore bottom, and these phe-nomena are independent of the hydration properties of pore wall, such as hydrophobic or hydrophilic.
Difference in metal growth direction between platinum and silver
Current mainly flows from the pore bottom when the electrodeposition is carried out on the porous silicon substrate. In addition, the resistivity of the microporous part is high. From these points of view, metal deposition should occur from the direction of the pore bottom to the opening. In fact, platinum deposition starts at the pore bottom of microporous structure in the present case. However, when silver electrodeposition is carried out on microporous silicon substrate, such growth does not appear, and silver deposition proceeds from the pore opening to the pore bottom (Figures 3 and 4). As dis-cussed below, the effect of displacement deposition occurring during electrodeposition and the different polarization behaviors on silicon and deposited metal can explain the difference in the growth direction.[image:3.595.57.539.463.685.2]
Electrodeposition is often accompanied by displacement deposition during noble metal electrodeposition in porous silicon. In case of platinum, the electrodeposition is prevailing compared to displacement deposition because the rate of platinum displacement deposition on silicon substrate is slow . Pore bottom is more favorable to electrodeposition than the opening in highly resistive microporous silicon, as mentioned above; hence, the
deposition proceeds from the direction of the pore bottom to the opening. This type of growth is observed for the hydrophobic porous silicon surface.
Figure 1a shows that platinum deposition on a silicon electrode needs much higher overpotential than that on a platinum electrode. Supposing that platinum depos-ition occurs on the top surface, the reaction preferen-tially proceeds on the top, and platinum is not deposited
inside the porous layer. In addition, it was reported that, when the nucleation of metal starts at the pore opening in the initial stage of the metal electrodeposition, the metal is preferentially deposited there, and the pore opening is plugged soon [1,2]. This type of growth is observed in porous silicon with the hydrophilic surface.[image:4.595.58.539.89.312.2] [image:4.595.58.539.473.695.2]
On the other hand, in case of silver, displacement de-position rate is extremely fast on silicon. Therefore, even Figure 3Cross-sectional views of microporous silicon after the electrodeposition of silver for 1 min.Images of (a,b) and (c,d) show the samples of hydrophilic and hydrophobic microporous silicon substrates, respectively. The images in (a) and (c) illustrate the SEI, and (b) and (d) illustrate the BEI.
though electrodeposition is carried out, displacement de-position proceeds preferentially compared to electrode-position. It was reported that metal displacement deposition proceeds from the pore opening to the pore bottom in the macroporous structure . Thus, silver electrodeposition also proceeds from the pore opening to the pore bottom in microporous structure because the effect of displacement deposition is stronger than that of electrodeposition. In addition, the potentials of silver deposition on the silicon electrode and silver elec-trode are similar (Figure 1b). These results show that, in the silver system, overpotential difference for silver elec-trodeposition on the silicon electrode and deposited sil-ver is sil-very small. Silsil-ver is deposited with almost equal rate on silver nuclei and bare silicon surface. The reac-tion does not preferentially proceed on the deposited surface at the pore opening. Therefore, pore opening is hard to be plugged, and silver ions can diffuse into the porous structure.
Why is silver not affected by property of the pore wall? Platinum is deposited within the hydrophobic micropor-ous silicon in Figure 2. However, when the pore wall is hydrophilic, platinum deposition occurs only on the top of the porous layer. These results can be explained by the affinity of the pore wall to water molecules. Platinum complex ion ([PtCl4]2−) behaves like a molecule with lower polarity due to its large size. Therefore, platinum ions have high affinity to the hydrophobic pore wall compared with water molecules to the pore wall, and hence, platinum ions are excluded from bulk to the pore wall . In case of platinum, platinum ions pass through a bare silicon surface because deposition proceeds to-ward the pore opening from the pore bottom. Therefore, platinum deposition behavior is affected by the hydra-tion property of pore wall. In hydrophilic microporous silicon, once deposition occurs at the pore opening, plat-inum is not deposited into pores but on the top surface due to the need of high overpotential on the bare silicon.
However, silver deposition is not affected by the hydra-tion properties of the pore wall. These results can be explained by the growth direction of deposition. Metal ions have to reach to the frontier of the deposition site and pass through not a bare silicon surface but the sur-face on which metal is deposited when metal deposition proceeds toward the pore bottom. Once the metal is deposited on the pore wall, the hydration property of pore wall changes due to the metal covering. Therefore, silver is uniformly deposited in microporous layer with-out relation to the hydration properties of the pore wall.
When the pore diameter of porous silicon is extremely small, platinum deposition is strongly affected by the hy-dration property of pore wall. On the other hand, silver deposition is not affected by the property. The results could be explained by the difference in overpotential be-tween the deposition on the metal surface and that on the silicon surface, and by the difference in intrinsic dis-placement deposition rate of metal. When metal electro-deposition is carried out in microporous silicon, the effect of the overpotential and the displacement depos-ition rate should be considered together with the hydra-tion property of the metal ions.
The authors declare that they have no competing interests.
We thank Prof. M Nakamura and Prof. H Takaya (Institute of Chemical Research, Kyoto University) for the help on experimental techniques and suggestions. This work was supported by Grant-in-Aid for Young Scientists (B) (grant no. 23750239).
RK and KF designed the experiments. RK carried out all the experimental work. TS and YHO supervised the work and joined the discussion. RK prepared the first draft of the manuscript. All authors read, revised, and approved the final manuscript.
RK is a PhD student in the Institute of Advanced Energy, Kyoto University. KF, TS and YHO are professors of the same university.
Received: 30 April 2012 Accepted: 21 June 2012 Published: 21 June 2012
1. Fukami K, Tanaka Y, Chourou ML, Sakka T, Ogata YH:Filling of mesoporous silicon with copper by electrodeposition from an aqueous solution.
2. Fang C, Foca E, Xu S, Carstensen J, Föll H:Deep silicon macropores filled with copper by electrodeposition.J Electrochem Soc2007,154:D45–D49. 3. Xu C, Zhang X, Tu K, Xie Y:Nickel displacement deposition of porous
silicon with ultrahigh aspect ratio.J Electrochem Soc2007,154:D170–D174. 4. Matsumoto T, Kobayashi K, Fukami K, Sakka T, Ogata YH:Electrodeposition
behavior of noble metals in ordered macroporous silicon.Phys Status Solidi C2009,6:1561–1565.
5. Fukami K, Kobayashi K, Matsumoto T, Kawamura YL, Sakka T, Ogata YH:
Electrodeposition of noble metals into ordered macropores in p-type silicon.J Electrochem Soc2008,155:D443–D448.
6. Fukami K, Koda R, Sakka T, Urata T, Amano K, Takaya H, Nakamura M, Ogata Y, Kinoshita M:Platinum electrodeposition in porous silicon: the influence of surface solvation effects on a chemical reaction in a nanospace.Chem Phys Lett2012,524:99-105.
7. Hamm D, Sakka T, Ogata YH:Transition during the growth of nanoporous columns in p-type silicon: the origin of macropores.Electrochemistry2003,
8. Imanishi A, Yamane S, Nakato Y:Si(111) surface modified with alpha, beta-unsaturated carboxyl groups studied by MIR-FTIR.Langmuir2008,